Journal of Hazardous Materials 163 (2009) 618–624
Contents lists available at ScienceDirect
Journal of Hazardous Materials journal homepage: www.elsevier.com/locate/jhazmat
Deﬂuoridation of water using magnesia/chitosan composite C. Sairam Sundaram a , Natrayasamy Viswanathan b , S. Meenakshi b,∗ a b
Department of Science and Humanities, Karaikal Polytechnic College, Karaikal 609609, Puducherry, India Department of Chemistry, Gandhigram Rural University, Gandhigram 624302, Tamilnadu, India
a r t i c l e
i n f o
Article history: Received 22 January 2008 Received in revised form 4 May 2008 Accepted 2 July 2008 Available online 11 July 2008 Keywords: MgO Chitosan MgOC composite Deﬂuoridation Adsorption
a b s t r a c t Magnesia (MgO) is a well-known adsorbent showing extremely high deﬂuoridation capacity (DC). In order to over come the limitations of MgO for ﬁeld applications, an attempt has been made to modify magnesia with abundant biomaterial chitosan to form magnesia/chitosan (MgOC) composite in a usable form and its merits over conventional magnesia and raw chitosan is established. Removal of ﬂuoride from aqueous solution with MgO and MgOC composite was studied with batch equilibrium experiments. At equilibrium, MgOC composite has a DC of 4440 mg F− /kg while for magnesia it is only 2175 mg F− /kg. The physicochemical properties of the synthesised MgOC composite were analyzed with FTIR and SEM with EDAX studies. The equilibrium data were ﬁtted with isotherm and kinetic models. Thermodynamic parameters viz, G◦ , H◦ and S◦ were calculated to understand the nature of sorption. Field studies were carried out to ﬁnd the suitability of these sorbents at ﬁeld conditions. © 2008 Elsevier B.V. All rights reserved.
1. Introduction Fluoride related health hazards are major environmental problems in many parts of the world. Excess of ﬂuoride in drinking water is harmful to human health. Various reports and studies established both the risks of high ﬂuoride dosing and beneﬁts of minimal exposure . The permissible limit of ﬂuoride concentration in drinking water is 1.5 mg/L as per WHO . Various deﬂuoridation technologies based on the principle of precipitation , ion exchange , adsorption  and electrochemical methods  have been proposed to remove excess ﬂuoride in drinking water and industrial efﬂuents. Among the methods, adsorption is considered as most suitable technique for ﬂuoride removal. Some adsorbents have been successfully used for the removal of ﬂuoride, including activated alumina , magnesia (MgO) , activated carbon , clay [10,11], rare earths , etc. However the most widely used and accepted sorbents are activated alumina and activated carbons in terms of ﬁeld applicability. Though MgO showed extremely high deﬂuoridation capacity (DC), it is not suitable for ﬁeld applications in view of its powder form as it would cause pressure drop and may affect ﬁltration during ﬁeld applications. Moreover, it needs one hour as the minimum contact time for maximum DC and pH of the treated water was found to be alkaline irrespective of the initial pH .
∗ Corresponding author. Tel.: +91 451 2452371; fax: +91 451 2454466. E-mail addresses: sairam [email protected]
(C. Sairam Sundaram), natrayasamy [email protected]
(N. Viswanathan), drs [email protected]
(S. Meenakshi). 0304-3894/$ – see front matter © 2008 Elsevier B.V. All rights reserved. doi:10.1016/j.jhazmat.2008.07.009
In the present study, in order to explore the possibility of utilizing the higher DC of MgO and to overcome its limitations, a biocomposite adsorbent which could be shaped into any desired form was prepared using MgO with chitosan, a biocompatible, nontoxic and biodegradable biopolymeric material. Chitosan has been recognised to remove cations and only a few reports are available about its capacity to remove anions [14–16]. Chitosan despite being abundant in nature, its adsorption ability has not been at satisfying level because chitosan ﬂakes/powder swells and crumbles and also has a tendency to form a gel in aqueous media. Although the amine and hydroxyl groups are responsible for adsorption, these active-binding sites are not readily available in gel or natural form. The adsorption capacity of the chitosan can be increased by spreading chitosan on physical supports that can increase the accessibility of the adsorbate-binding sites . Hence chitosan has been selected for the preparation of composites with magnesia. The studies have been conducted on the optimisation of various experimental conditions like pH, dosage, different initial ﬂuoride concentrations, inﬂuence of competitor anions and the effect of temperatures on ﬂuoride sorption. The DC of MgOC composite was compared with that of MgO and chitosan. The advantages of using MgOC composite over MgO and chitosan as a deﬂuoridation agent have been established. The mechanism of ﬂuoride removal is reasonably explained by adsorption isotherms. The nature and morphology of the sorbents are discussed on the basis of SEM with EDAX and FTIR studies. Various kinetic models including pseudo-ﬁrst-order, pseudo-second-order, particle diffusion and intraparticle diffusion models were used to describe the adsorption process. The sorbents were tested with a ﬁeld sample collected in
C. Sairam Sundaram et al. / Journal of Hazardous Materials 163 (2009) 618–624
a nearby ﬂuoride-endemic village for their suitability under ﬁeld conditions. 2. Experimental 2.1. Synthesis of MgOC composite Chitosan was purchased from Pelican Biotech and Chemicals Labs, Kerala (India). Its degree of deacetylation is 85%. MgO and all other chemicals used were of analytical reagent grade and used without further puriﬁcation. The synthesis of MgOC composite was carried out by mixing magnesium oxide and chitosan in the ratio 3:2 and the aqueous mixture was kept for 24 h and ﬁltered. Then the mixture was dried at 80 ◦ C in an oven and calcined at 400 ◦ C to get MgOC composite . 2.2. Adsorption studies Batch technique was selected to obtain the equilibrium and kinetic data. Stock ﬂuoride solution (100 mg/L) was prepared by dissolving 0.221 g of anhydrous sodium ﬂuoride in 1 L distilled water and was further diluted to get the desired concentration . About 0.1 g of sorbent was added to 50 ml of solution containing 10 mg/L as initial ﬂuoride concentration. The mixture was shaken in a thermostated shaker at a speed of 200 rpm at room temperature. The effect of different initial ﬂuoride concentrations at three different temperatures viz., 303, 313 and 323 K on sorption rate was studied by keeping the mass of sorbent as 0.1 g and volume of solution as 50 ml in neutral pH. The ﬂuoride concentration was measured using expandable ion analyzer EA 940 and the ﬂuoride ion selective electrode BN 9609 (Orion, USA). The pH measurements were carried out with the same instrument with pH electrode. All other water quality parameters were analyzed by using standard methods . The pH at zero point charge (pHzpc ) of sorbents was measured using the pH drift method . 2.3. Instrumental studies The surface morphological studies of treated and raw samples were characterised using SEM with EDAX HITACHI-S-3400H model. FTIR spectra of both treated and raw samples were characterised using JASCO-460 plus model FTIR spectrophotometer to detect the functional groups. The speciﬁc surface area of the composite was analyzed using BET isotherm method with NOVA 1000 model. Computations were made using Microcal Origin (Version 6.0) software. The goodness of ﬁt was discussed using regression correlation coefﬁcient (r) and 2 -analysis. 3. Results and discussion 3.1. Characterisation of the composite The speciﬁc surface area of MgOC composite was found to be 45.5143 m2 /g. FTIR spectrum is a useful tool to identify functional groups in a molecule, as each speciﬁc chemical bond often has a unique energy absorption band and can obtain structure, bond information, study of strength and fraction of hydrogen bonding. FTIR spectra of MgOC composite before and after treated with ﬂuoride were given in Fig. 1a and b. The band at 3700 cm−1 corresponds to –OH stretching vibration. Although there is a possibility of overlapping between –NH2 and –OH stretching vibrations, the band 3437 cm−1 corresponds to –OH and –NH2 stretching vibrations. The band at 1660 cm−1 corresponds to amide stretching vibration .
Fig. 1. FTIR spectra of (a) MgOC composite and (b) ﬂuoride-sorbed MgOC composite.
The bands at 2929 and 1430 cm−1 corresponds to aliphatic stretching vibrations of –CH and –NH bending vibrations of chitosan, respectively. The slight broadening of –OH stretching vibration band at 3437 cm−1 in the ﬂuoride-sorbed MgOC composite when compared with MgOC composite corresponds to the formation of O–H· · ·F bond  which conﬁrms the existence of hydrogen bonding. The changes in the surface of the MgOC composite before and after sorbed with ﬂuoride was identiﬁed by SEM micrographs and are presented in Fig. 2a and b, respectively. The presence of relevant elements in MgOC composite was conﬁrmed by their respective peaks (cf. Fig. 2c). The presence of ﬂuoride peak in the EDAX spectra of ﬂuoride treated MgOC composite conﬁrms the ﬂuoride sorption which is shown in Fig. 2d. The surface morphological changes of magnesia and MgOC composite were also conﬁrmed by the shifting of pHzpc values . The pHzpc of MgO is 10.0 where as for MgOC composite this value shifted to 10.6 which clearly indicate the occurrence of structural changes in the composite (cf. Fig. 3). 3.2. Effect of contact time Fig. 4 shows the effect of contact time on the removal of ﬂuoride by chitosan, MgO and MgOC composite for an initial ﬂuoride concentration of 10 mg/L. The rate of ﬂuoride removal was rapid initially and gradually it attained equilibrium. It is quite interesting to note that the MgOC composite reached saturation at 30 min whereas for MgO it was rather slow and attained equilibrium only after 60 min. The DC of MgOC composite (4440 mgF− /kg) is also very high which is just double than that of MgO (2175 mgF− /kg). As raw chitosan experienced a minimum DC (52 mgF− /kg), further studies were carried out with MgOC composite and MgO for comparison. Based on these observations, for subsequent experiments the shaking time was ﬁxed as 30 min for MgOC composite and 60 min for MgO. 3.3. Effect of sorbent dosage on ﬂuoride sorption The effect of the adsorbent dosage of both MgO and its chitosan composite MgOC is carried out with an initial ﬂuoride concentration of 10 mg/L and shown in Fig. 5. It is observed that the percentage ﬂuoride removal increased with the increase in the dosage of the sorbent in both cases and it is obvious due to the
C. Sairam Sundaram et al. / Journal of Hazardous Materials 163 (2009) 618–624
Fig. 2. SEM images of (a) MgOC composite and (b) ﬂuoride-sorbed MgOC composite, EDAX spectra of (c) MgOC composite and (d) ﬂuoride-sorbed MgOC composite.
enhanced active sites with an increase in the amount of sorbent . The percent removal of ﬂuoride by MgOC composite is higher when compared to MgO. For 0.1 g of MgOC composite, the percent removal is 91% and for MgO it is 40%. However to make a comparative study, 0.1 g was ﬁxed as optimum dosage for both MgO and MgOC composite.
Fig. 3. pHzpc of the sorbents.
3.4. Inﬂuence of pH The sorption of ﬂuoride from aqueous solution was highly dependent on the solution pH, as it altered the surface charge on the sorbent. Fig. 6 shows sorption of ﬂuoride using MgO and MgOC composite as a function of pH with an initial ﬂuoride concentration of 10 mg/L at 303 K. It was observed that there is no marked
Fig. 4. Effect of DC of sorbents with contact time.
C. Sairam Sundaram et al. / Journal of Hazardous Materials 163 (2009) 618–624
Fig. 5. Effect of dosage of sorbents in the percent removal.
difference in DC of both sorbents at different pH environment and concluded that the DC was not inﬂuenced by the pH of the medium. However the pH of the treated water was found to be alkaline irrespective of the initial pH and it is obvious as the material itself is basic in nature. The pH of the treated water samples in both cases falls in between 10.1 and 10.4.
3.5. Effect of initial ﬂuoride concentration The adsorption of ﬂuoride onto MgO and MgOC composite with various initial ﬂuoride concentrations ranging from 10 to 23 mg/L were carried out and presented in Fig. 7. It is observed that the DC of both the sorbents increases with increase in initial ﬂuoride concentration. Similar results were reported by Lv et al.  while studying ﬂuoride sorption on layered double hydroxides. It can also be inferred that the ﬂuoride removal is signiﬁcant at higher concentrations in both cases. However the DC of MgOC composite is higher when compared to MgO. As the MgOC composite has higher DC than that of MgO, further studies were limited to with MgOC composite.
Fig. 6. Inﬂuence of pH.
Fig. 7. Effect of DC with different initial ﬂuoride concentrations.
3.6. Effect of other anions The ﬂuoride-contaminated drinking water may contain several other anions which may compete with the sorption of ﬂuoride. The DC of MgOC composite was experimentally veriﬁed in the presence of other common anions like Cl− , SO4 2− , NO3 − and HCO3 − was investigated with varying initial concentrations of these ions ranging from 100 to 500 mg/L by keeping 10 mg/L as initial ﬂuoride concentration at 303 K. Fig. 8 shows the inﬂuence of other anions in the DC of MgOC composite. There is a slight increase in the DC of MgOC composite in the presence of Cl− , SO4 2− and NO3 − ions, but the DC decreases in presence of HCO3 − ions. This is due to the competition of bicarbonate ions with ﬂuoride ions in the sorption process. Parallel interference of bicarbonate ions on the DC has been cited earlier by Karthikeyan et al.  while using montmorillonite adsorbent for ﬂuoride removal. 3.7. Sorption isotherms To quantify the sorption capacity of the MgOC composite for the removal of ﬂuoride, two isotherms namely Freundlich and Langmuir have been adopted.
Fig. 8. Effect of other anions in the DC of MgOC composite.
C. Sairam Sundaram et al. / Journal of Hazardous Materials 163 (2009) 618–624 Table 3 Thermodynamic parameters
Table 1 Isotherms and their linear forms Isotherms
1/n Freundlich qe = kF Ce o bC e Langmuir qe = Q 1+bCe
log qe = log kF + Ce qe
1 n log Ce
log qe vs. log Ce Ce qe
3.7.1. Freundlich isotherm The linear form of Freundlich isotherm  is given in Table 1. The linear plot of log qe vs. log Ce indicates the applicability of Freundlich isotherm. The constants kF and 1/n relates to the measure of adsorption capacity and adsorption intensity, respectively. These constants of Freundlich isotherm of MgOC composite is given in Table 2. Values of 1/n are lying between 0 and 1 and the n-value lying in the range of 1–10 conﬁrms the favorable conditions for adsorption . The adsorption capacity kF increases with increase in temperature suggesting that the ﬂuoride uptake by MgOC composite is an endothermic process.
Standard free energy Standard enthalpy change Standard entropy change
ln(qe /Ce ) vs. Ce ln Ko vs. 1/T
= −RT ln Ko ln Ko = o H o + S RT R
Table 4 Thermodynamic parameters of ﬂuoride sorption on MgOC composite Thermodynamic parameters
Go (kJ mol−1 ) 303 K 313 K 323 K
−1456.15 −1057.74 −629.62
Ho (kJ mol−1 ) So (kJ mol−1 K−1 )
3.8. Thermodynamic treatment of the sorption process 3.7.2. Langmuir isotherm The linear form of Langmuir isotherm  is represented in Table 1. The Langmuir constants Qo and b are related to sorption capacity and sorption energy, respectively. Maximum sorption capacity (Qo ) represents monolayer coverage of sorbent with sorbate and b represents the energy of sorption and should vary with temperature. The linear plot of Ce /qe vs. Ce indicates the applicability of Langmuir isotherm. The values of Langmuir constants are given in Table 2. In order to ﬁnd out the feasibility of the isotherm, the essential characteristics of the Langmuir isotherm can be expressed in terms of a dimensionless constant separation factor or equilibrium parameter, RL  RL =
1 1 + bCo
where b is the Langmuir isotherm constant and Co is the initial concentration of ﬂuoride (mg/L). The RL -values between 0 and 1 indicate favorable adsorption for all the temperatures studied (cf. Table 2). 3.7.3. 2 -analysis To identify a suitable isotherm model for the sorption of ﬂuoride on MgOC composite, this analysis has been carried out. The equivalent mathematical statement is 2 =
(qe − qe,m )2
where qe,m is equilibrium capacity obtained by calculating from the model (mg/g) and qe is experimental data of the equilibrium capacity (mg/g). If data from the model are similar to the experimental data, 2 will be a small number, while if they differ, 2 will be a bigger number. Therefore, it is also necessary to analyze the data set using the non-linear 2 -test to conﬁrm the best-ﬁt isotherm for the sorption system . The results of 2 -analysis are presented in Table 2. The lower 2 -values of Freundlich isotherm indicate the better applicability for the ﬂuoride sorption on MgOC composite.
Thermodynamic parameters associated with the adsorption, viz., standard free energy change (G◦ ), standard enthalpy change (H◦ ) and standard entropy change (S◦ ) were calculated [5,28] using the equations given in Table 3. The values of thermodynamic parameters are shown in Table 4. The negative values of G◦ conﬁrm the feasibility and the spontaneous nature of ﬂuoride sorption. The value of H◦ is positive indicating that the sorption reaction is endothermic. The positive value of S◦ which is a measure of randomness at the solid/liquid interface during ﬂuoride sorption indicates the sorption process is irreversible and stable. 3.9. Sorption kinetic models The two main types of sorption kinetic models namely reaction-based and diffusion-based models were adopted to ﬁt the experimental data . The study of sorption dynamics describes the solute uptake rate and evidently this rate controls the residence time of adsorbate uptake at the solid/solution interface. A relatively higher r-value indicates that the model successfully describes the kinetics of sorption of ﬂuoride on the sorbent. 3.9.1. Reaction-based models The most commonly used pseudo-ﬁrst-order and pseudosecond-order models were employed to explain the solid/liquid adsorption. A simple pseudo-ﬁrst-order kinetic model  is represented in Table 5. The slope of the straight-line plot of log (qe − qt ) against t for different experimental conditions will give the value of the rate constants (kad ) and are given in Table 6. There are four types of linear pseudo-second-order kinetic models , the most popular linear form is given in Table 5. The ﬁtness of the data and the values of qe , k, and h were obtained from the plots of t/qt vs. t for ﬂuoride sorption at different temperatures viz., 303, 313 and 323 K of MgOC composite is presented in Table 6. The plot of t/qt vs. t gives a straight-line with higher correlation coefﬁcient r-values which is higher than that observed with pseudo-ﬁrst-order model indicating the applicability of pseudo-second-order model.
Table 2 Freundlich and Langmuir isotherm parameters of ﬂuoride sorption on MgOC composite with r- and 2 -values Temperature (K)
303 313 323
kF (mg/g) (L/mg) 1/n
0.169 0.161 0.145
5.917 6.211 6.897
8.472 8.810 9.141
0.970 0.960 0.952
0.003 0.005 0.006
11.236 11.364 11.494
2.967 3.520 4.350
0.019 0.016 0.013
0.996 0.995 0.995
0.012 0.018 0.025
C. Sairam Sundaram et al. / Journal of Hazardous Materials 163 (2009) 618–624 Table 7 Field trial results of the sorbents
Table 5 Kinetic models and their linear forms Kinetic models
Water quality parameters
log(qe − qt ) vs. t t qt vs. t
F− (mg/L) pH Cl− (mg/L) Total hardness (mg/L) Total dissolved solids (mg/L) Na+ (mg/L) K+ (mg/L)
4.13 9.60 85.20 240.00 2400.00 173.00 23.00
Reaction-based log(qe − qt ) = log qe − t 1 t qt = h + q e
Ct Ce t1/2
ln 1 −
q t = ki
kad t 2.303
= −kp t
Ct Ce t1/2
ln 1 − qt vs.
After treatment MgO
3.44 10.12 85.20 220.00 2270.00 173.00 22.00
0.66 10.10 81.60 210.00 2190.00 172.00 21.00
which indicates that both the materials have their zero point charge at this pH levels, which in turn suggesting that the sorbents possesses positive charge upto this pH values and hence the positively charged surface of the sorbents removes ﬂuoride by means of electrostatic attraction for a wide pH range. The higher DC of MgOC composite may be attributed to the fact that chitosan also contribute in the enhancement of DC by removing ﬂuoride through hydrogen bonding [17,21,34]. 3.11. Field trial
Fig. 9. Mechanism of ﬂuoride sorption on MgO and MgOC composite.
3.9.2. Diffusion-based models For a solid–liquid sorption process, the solute transfer is usually characterised either by particle diffusion or intraparticle diffusion control. A simple equation for the particle diffusion controlled sorption process [5,32] is given in Table 5. The intraparticle diffusion model used here refers to the theory proposed by Weber and Morris . The intraparticle diffusion equation is given in Table 5. The straight-line plots of ln(1 − Ct /Ce ) vs. t and qt vs. t0.5 indicates the applicability of both particle and intraparticle diffusion models. The kp , ki and r-values of particle and intraparticle diffusion models are illustrated in Table 6. The higher r-values obtained for both particle and intraparticle diffusion models suggest that MgOC composite follow both the models on ﬂuoride sorption. 3.10. Mechanism of ﬂuoride removal The mechanism of ﬂuoride removal of both MgO and MgOC composite was mainly governed by adsorption and is illustrated in Fig. 9. Interestingly, both the sorbents has little or no effect with the change in the pH of the environment. The pHzpc values of MgO and MgOC composite happened to be at 10 and 10.6, respectively,
The sorbents used in our study are also tested with ﬁeld sample taken in a nearby ﬂuoride-endemic village. About 1.0 g of sorbent was added to 50 ml of ﬂuoride water sample and the contents were shaken with constant time at room temperature. These results are presented in Table 7. The ﬁeld trial results suggest that these sorbents can be effectively used as deﬂuoridating agents at the ﬁeld level. There is a signiﬁcant reduction in the levels of other water quality parameters also in addition to ﬂuoride. 4. Conclusions In the present study, a novel adsorbent namely MgOC composite was prepared to remove ﬂuoride from drinking water which possesses an appreciable higher DC than magnesia. The DC of both the sorbents is not inﬂuenced by pH of the medium. The DC of MgOC composite was not affected in the presence of co-anions except bicarbonate ion. The sorption process follows Freundlich isotherm. The thermodynamic parameter values indicate that the ﬂuoride removal process is spontaneous and endothermic in nature. The kinetics of MgOC composite follows pseudo-second-order, particle and intraparticle diffusion models. The results of ﬁeld trial indicate that both the sorbents can be effectively used to remove ﬂuoride from water. However the treated water found to be alkaline in nature when both the sorbents were used as the deﬂuoridating medium. Among the two adsorbents, MgOC composite being biocompatible, biodegradable, cost effective, shaped into
Table 6 The parameters of various kinetic models with r-values Kinetic models
qe (mg/g) k (g/mg min) h (mg/g min) r
0.804 0.412 0.266 0.996
0.961 0.670 0.618 0.999
1.098 0.452 0.545 0.999
1.068 0.479 0.546 0.999
0.881 0.613 0.475 0.999
1.034 0.652 0.698 0.999
1.101 0.735 0.891 0.999
1.115 0.460 0.572 0.999
0.915 1.034 0.865 1.00
1.046 1.125 1.230 0.999
1.162 0.441 0.596 0.998
1.252 0.315 0.494 0.998
kp (min−1 ) r
ki (mg/g min0.5 ) r
C. Sairam Sundaram et al. / Journal of Hazardous Materials 163 (2009) 618–624
any desired form which possesses higher DC with minimum contact time and can be used as a promising sorbent for ﬂuoride removal. Acknowledgement The authors are thankful to University Grants Commission, New Delhi, India for the provision of support to carry out this research work. References  M. Hichour, F. Persin, J. Sandeaux, C. Gavach, Fluoride removal from waters by Donnan dialysis, Sep. Purif. Technol. 18 (2000) 1–11.  WHO Report, Fluoride and Fluorides: Environmental Health Criteria, World Health Organisation, 1984.  K.R. Bulusu, B.B. Sundaresan, B.N. Pathak, W.G. Nawlakhe, D.N. Kulkarni, V.P. Thergoankar, Fluorides in water, deﬂuoridation methods and their limitation, J. Inst. Eng. Environ. Eng. Div. 60 (1979) 1–25.  K.M. Popat, P.S. Anand, B.D. Dasare, Selective removal of ﬂuoride ions from water by the aluminium form of the aminomethylphosphonic acid-type ion exchanger, React. Polym. 23 (1994) 23–32.  S. Meeenakshi, N. Viswanathan, Identiﬁcation of selective ion exchange resin for ﬂuoride sorption, J. Colloid Interface Sci. 308 (2007) 438–450.  S.K. Adhikary, U.K. Tipnis, W.P. Harkare, K.P. Govindan, Deﬂuoridation during desalination of brackish water by electrodialysis, Desalination 71 (1989) 301–312.  Y. Ku, H.M. Chiou, The adsorption of ﬂuoride ion by activated alumina, Water Air Soil Pollut. 133 (2002) 349–360.  V.P. Thergoankar, W.G. Nawlakhe, Activated magnesia for ﬂuoride removal, Ind. J. Environ. Health 16 (1971) 241–243.  R. Mckee, W.S. Johnston, Removal of ﬂuoride by low cost adsorbents, Ind. J. Environ. Health 41 (1999) 53–58.  G. Karthikeyan, A. Pius, G. Alagumuthu, Fluoride adsorption studies of montmorillonite clay, Indian J. Chem. Technol. 12 (2005) 263–272.  Y. Cengeloglu, K. Esengul, M. Ersoz, Removal of ﬂuoride from aqueous solution by using red mud, Sep. Sci. Technol. 28 (2002) 81–86.  A.M. Raichur, M. Jyoti Basu, Adsorption of ﬂuoride onto mixed rare earth oxides, Sep. Purif. Technol. 24 (2001) 121–127.  V.P. Thergaonkar, W.G. Nawalakhe, Activated magnesia for ﬂuoride removal, Ind. J. Environ. Health 16 (1971) 241–243.  W. Ma, F.Q. Ya, M. Han, R. Wang, Characteristics of equilibrium, kinetics studies for adsorption of ﬂuoride on magnetic–chitosan particle, J. Hazard. Mater. 143 (2007) 296–302.
 S.P. Kamble, S. Jagtap, N.K. Labhsetwar, D. Thakare, S. Godfrey, S. Devotta, S.S. Rayalu, Deﬂuoridation of drinking water using chitin, chitosan and lanthanummodiﬁed chitosan, Chem. Eng. J. 129 (2007) 173–180.  K. Jaafari, S. Elmaleh, J. Coma, K. Benkhouja, Equilibrium and kinetics of nitrate removal by protonated cross-linked chitosan, Water SA 27 (2001) 9–13.  D. Zhou, M. He, Y. Zhang, M. Huang, Y. Jiang, Asymmetric hydrogenation of diketones catalyzed by magnesium oxide supported chitosan–Rh complex, Polym. Adv. Technol. 14 (2003) 287–291.  F. Chen, Z.C. Wang, C.J. Lin, Preparation and characterization of nano-sized hydroxyapatite particles and hydroxyapatite/chitosan nano-composite for use in biomedical materials, Mater. Lett. 57 (2002) 856–861.  APHA, Standard Methods for the Examination of Water and Waste Water, American Public Health Association, Washington, DC, 2005.  M.V. Lopez-Ramon, F. Stoeckli, C. Moreno-Castilla, F. Carrasco-Marin, On the characterization of acidic and basic surface sites on carbons by various techniques, Carbon 37 (1999) 1215–1221.  D. Zhou, L. Zhang, S. Guo, Mechanisms of lead biosorption on cellulose/chitin beads, Water Res. 39 (2005) 3755–3762.  Y.S. Al-Degs, M.I. El-Barghouthi, A.A. Issa, M.A. Khraisheh, G.M. Walker, Sorption of Zn(II), Pb(II) and Co(II) using natural sorbents: equilibrium and kinetic studies, Water Res. 40 (2006) 2645–2658.  A. Mellah, S. Chegrouche, The removal of zinc from aqueous solutions by natural bentonite, Water Res. 31 (1997) 621–629.  L. Lv, J. He, M. Wei, D.G. Evans, Z. Zhou, Treatment of high ﬂuoride concentration water by MgAl-CO3 layered double hydroxides: kinetic and equilibrium studies, Water Res. 41 (2007) 1534–1542.  H.M.F. Freundlich, Über die adsorption in lösungen, Z. Phys. Chem. 57A (1906) 385–470.  I. Langmuir, The constitution and fundamental properties of solids and liquids, J. Am. Chem. Soc. 38 (1916) 2221–2295.  T.W. Weber, R.K. Chakravorti, Pore and solid diffusion models for ﬁxed bed adsorbers, J. Am. Inst. Chem. Eng. 20 (1974) 228–238.  A.A. Khan, R.P. Singh, Adsorption thermodynamics of carbofuran on Sn (IV) arsenosilicate in H+ , Na+ and Ca2+ forms, Colloids Surf. 24 (1987) 33–42.  Y.S. Ho, J.C.Y. Ng, G. McKay, Kinetics of pollutant sorption by biosorbents: review, Sep. Purif. Methods 29 (2000) 189–232.  S. Lagergren, Zur theorie der sogenannten adsorption gelöster stoffe, K. Sven. Vetenskapsakad. Handl. 24 (1898) 1–39.  Y.S. Ho, Second order kinetic model for the sorption of cadmium onto tree fern: a comparison of linear and non linear methods, Water Res. 40 (2006) 119–125.  D. Wankasi, M. Horsfall, A.I. Spiff, Retention of Pb (II) ion from aqueous solution by nipah palm (nypa fruticans wurmb) petiole biomass, J. Chil. Chem. Soc. 50 (2005) 691–696.  W.J. Weber, J.C. Morris, Equilibria and capacities for adsorption on carbon, J. Sanitary Eng. Div. 90 (1964) 79–91.  Y. Nakano, K. Takeshita, T. Tsutsumi, Adsorption mechanism of hexavalent chromium by redox with condensed-tannin gel, Water Res. 35 (2001) 496–500.